{'fraction_non_alphanumeric': 0.0291361232253874, 'fraction_numerical': 0.016887816646562123, 'mean_word_length': 4.974223946784923, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 6, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Covalent functionalization of polypropylene filters with diazirine–photosensitizer conjugates producing visible light driven virus inactivating materials﻿

The SARS-CoV-2 pandemic has highlighted the weaknesses of relying on single-use mask and respirator personal protective equipment (PPE) and the global supply chain that supports this market. There have been no major innovations in filter technology for PPE in the past two decades. Non-woven textiles used for filtering PPE are single-use products in the healthcare environment; use and protection is focused on preventing infection from airborne or aerosolized pathogens such as Influenza A virus or SARS-CoV-2. Recently, C–H bond activation under mild and controllable conditions was reported for crosslinking commodity aliphatic polymers such as polyethylene and polypropylene. Significantly, these are the same types of polymers used in PPE filtration systems. In this report, we take advantage of this C–H insertion method to covalently attach a photosensitizing zinc-porphyrin to the surface of a melt-blow non-woven textile filter material. With the photosensitizer covalently attached to the surface of the textile, illumination with visible light was expected to produce oxidizing 1O2/ROS at the surface of the material that would result in pathogen inactivation. The filter was tested for its ability to inactivate Influenza A virus, an enveloped RNA virus similar to SARS-CoV-2, over a period of four hours with illumination of high intensity visible light. The photosensitizer-functionalized polypropylene filter inactivated our model virus by 99.99% in comparison to a control.

www.nature.com/scientificreports/ An alternative approach to PPE reuse is to modify the base materials. Ideally, the materials possess filtering, continuous pathogen inactivation, and the ability to self-sterilize when exposed to a plentiful and accessible stimulus. Light is a stimulus that is abundant from both natural and synthetic sources, accessible, and relatively low in cost. Photodynamic therapy (PDT) is a technology that utilizes light (including within the visible spectrum) and photosensitizing (PS) molecules to eradicate pathogens, reduce infection, or eliminate unwanted or cancerous tissue through the production and reaction of singlet oxygen ( 1 O 2 ) and/or reactive oxygen species (ROS) 13,14 . PDT has been used extensively in vivo and can be used without causing undue bodily harm 14 . When illuminated with visible light the photosensitizer is excited and proceeds through an energy transfer process with abundant triplet oxygen ( 3 O 2 ) to produce 1 O 2 and ROS locally that can be used to eliminate pathogens. The activity is non-specific and can eliminate resistant pathogens that are typically difficult to eradicate [15][16][17] . As an added benefit, pathogens cannot evolve resistance to 1 O 2 as easily as they can to small molecule inhibitors 15,17 .
Polymer composites, natural and synthetic polymers, and silica particles have been covalently functionalized with photosensitizing molecules and used for microbial inactivation, with the majority of applications focusing on bacterial inactivation 18 . Non-covalent impregnation of photosensitizers into bulk polymer matrices has also been demonstrated to result in microbial inactivation 19 , but the lack of covalent attachment within these systems may lead to leaching of the photosensitizer into the environment. As a result, larger concentrations of the additive will be required in order to avoid a decrease in surface concentration-and therefore activity-over time. Furthermore, the leaching of active components can impact human and environmental health.
Covalent attachment approaches have the advantage of reducing the possibility of active component release (leaching) which would inevitably result in a decrease in performance over time. In addition, covalent attachment of photosensitizers can allow the surface of a material to be modified without affecting the bulk. This places the photosensitizer where it is needed (since only the surface of a material can interact with pathogens), thereby requiring less agent to achieve a desired response. In addition, the bulk properties of the substrate material (e.g. tensile strength or glass transition temperature) will be left unperturbed.
Rose Bengal, methylene blue, ruthenium-based complexes, pthalocyanines, and porphyrins have been covalently attached to natural and synthetic polymers that bear suitable chemical functionality to support the occurrence of chemical reactions at their surface [20][21][22][23][24][25][26][27][28][29] . These covalent attachment methods have been specifically designed for high-functionality materials that are not typically used in PPE/healthcare settings, or else require material pre-functionalization to allow 'click chemistry' (i.e. azide-alkyne coupling through Huisgen cycloadditions). A general solution for attaching photosensitizing molecules onto non-functional materials, such as aliphatic polymers used in PPE for example, remains an obstacle. These types of materials are comprised entirely of C-C and C-H bonds, and therefore lack any chemical "handles" that can be used for derivatization with photosensitizers.
One of our research groups recently described a family of bis-diazirine reagents that can be used to crosslink simple aliphatic polymers like polyethylene and polypropylene 30,31 . The reagents work by expelling nitrogen gas (N 2 ) from the tethered diazirine groups upon thermal or photochemical stimulation, to afford high-energy carbenes which can then undergo rapid, low-barrier insertion into any available C-H bonds. In principle, such a technique can also be used to add functionality to base polymeric materials: the desired functional group can simply be tethered to one or more diazirine units, and the resulting conjugate can then be irreversibly linked to the surface of any polymeric material through appropriate activation of the diazirine function.
Herein, we employ this C-H activation strategy to permit the covalent functionalization of non-woven melt-blown polypropylene textiles with a common photoactive molecule (Fig. 1). The combination of different melt-blown polypropylene non-woven filters are what make up most surgical and N95 respirators; the cover layer, commonly called spun-bond polypropylene (SBPP) has a fiber density of ~ 15 g/m 2 ; and the filter, commonly called, simply, melt-blown polypropylene (MBPP) has a density of ~ 30 g/m 2 . The lack of functional groups in this material means that it cannot be derivatized by traditional covalent linking methods. As a proof of concept, we demonstrated the inactivation of influenza A virus (IFV) using a visible light stimulus. IFV was chosen as a model because IFV itself is a major threat as a potential pandemic virus, and because IFV's enveloped structure and RNA genome are similar to those of SARS-CoV-2-the organism that is the proximal cause of the current pandemic. Researchers have indicated previously the importance of developing and testing inactivation methods against enveloped viruses, given that a pandemic was expected long before the emergence of SARS-CoV-2 32 . www.nature.com/scientificreports/

Results and discussion
Functionalization of non-woven polypropylene filter with photoactive porphyrin. The SBPP and MBPP substrates were chosen because of the widespread use of the non-woven material in filtering PPE, specifically single-use surgical masks and N95/personal air purifying respirators. A commercially available photosensitizer (1) was selected, which possessed a high quantum yield for the production of singlet oxygen with visible light, and which possessed nucleophilic residues for easy derivatization. To facilitate insertion into the surface accessible C-H bonds of the SBPP and MBPP, we utilized a 3-trifluoromethyl-3-phenyl-3H-diazirine motif (TFPD) that is known to generate carbenes that are capable of ready insertion into C-H bonds 33 . A commercially available benzyl bromide (2) that incorporates the TFPD motif was reacted with the pyridyl groups of 1 to produce the desired tetrakis diazirinyl zinc-porphyrin 3 in near-quantitative yield (Fig. 2a). We www.nature.com/scientificreports/ at 1273 nm. The 1 O 2 generation proceeds through the photoexcitation of ground state 3 (S 0 ) to generate the singlet excited state of 3 (S 1 ), intersystem crossing to a triple state 3 (T 3 ), and then an energy transfer to the triplet ground state of oxygen ( 3 O 2 ) to produce singlet oxygen ( 1 O 2 ) which then undergoes phosphorescence back to the ground state observed as an emission at a wavelength of 1273 nm indicating that the zinc-porphyrin moiety still possessed activity when functionalized with four diazirine groups (Fig. 2b). The surface of the SBPP and MBPP were then covalently functionalized with 3 using a modified procedure from Lepage et al. 30 To facilitate this, the reactivity of the diazirines in 3 was first analyzed by differential scanning calorimetry (DSC). These data revealed an onset temperature of 108 °C (determined by extrapolation of the tangent of the upward slope to the fitted baseline of the plot) and a peak temperature of 137 °C (Fig. 2c). With this information in hand, we chose to react compound 3 with SBPP and MBPP for 4 h at 120 °C (using 10 wt% of 3 with respect to SBPP or MBPP) to afford SBPP-3 and MBPP-3, green-coloured textiles. The lower density textile SBPP (and subsequent functionalized SBPP-3) was used exclusively herein to test virus inactivation and quantify ROS/ 1 O 2 production. The higher density textile MBPP (and subsequent functionalized MBPP-3) was used to analyze the effect on filtration performance.
The intense green colour of 3 was advantageous for (1) ensuring coverage of SBPP (and MBPP in an analogous procedure) with the solution of 3, and (2) monitoring the effectiveness of the diazirine C-H insertion reaction through the persistent green colour after washing (Fig. S5). The surfaces of MBPP in comparison to MBPP-3 were imaged by scanning electron microscopy, which confirmed that there was no observable change to the surface of the fibers (Supplementary Fig. S6).
Prior to virus inactivation testing we completed a robust washing protocol analyzing the wash fractions with UV-Vis spectroscopy to observe the removal of 3 that did not covalently react with the surface of SBPP. The washing process was initially completed over ~ 6 days with 12 changes in solvent (Fig. S4). It was crucial to ensure complete removal of any 3 that did not covalently bind to SBPP during the C-H insertion step, to ensure that our subsequent virus inactivation testing focused on the abilities of SBPP-3 exclusively. The efficacy of free antimicrobials is greater than that of an immobilized antimicrobial because of the ability to diffuse throughout a solution; in the case of an immobilized antimicrobial, the activity is reliant upon virus diffusion to within the proximity of the surface of the material where the interaction/reaction can occur. The lifetime of the 1 O 2 /ROS produced (µs to ms) limits the space in which inactivation may take place, which we hypothesized would create a layer at and above the material's surface that would inactivate any virus occupying that space 34,35 . The inactivation would then rely on pathogen diffusion in the transfer medium to within this concentrated 1 O 2 area on the SBPP-3 surface and was therefore expected to present a time-dependence. Virus inactivation testing was then completed using SBPP-3 using a minimal volume of carrier medium to mimic aerosolized and droplet capture by the filter.
IFV (strain A/California/07/2009) was used as a model enveloped RNA virus. IFV would provide insight into the inactivation performance of our material against enveloped RNA viruses similar to the SARS-CoV-2, which continues to cause a worldwide pandemic in 2021. We used a high-intensity LED light capable of producing ~ 30,000 lx to excite SBPP-3 (see Supplementary Fig. 7 for manufacturer's provided UV-Vis profile) which would mimic the amount of light that may be found in a hospital operating theatre or emergency area 36 .
The virus particles were exposed to the light for between 0.5 and 4 h in 10 µL of tissue culture medium in a well of a 96-well plate that contained a test surface (see Supplementary Fig. S5). After 1 h exposure the virus titer was reduced by 1.06 log with SBPP-3, compared with only a minor 0.13 log reduction on the SBPP control surface (Fig. 3a). Over the 4-h testing period a logarithmic relationship between reduction of PFUs and exposure time was observed. At 4 h of exposure, the treated surface resulted in a 4.07 log reduction (99.99%) in comparison to an empty well, a 3.38 log reduction (99.96%) in comparison to untreated SBPP and a 5.95 log reduction (99.9999%) in comparison to the starting virus PFU concentration.
These data indicate that near-sterilization levels of inactivation may be achievable over longer periods (4 + hours) of high-intensity illumination of SBPP-3, offering an alternative approach to re-sterilization and re-use of PPE. A distinct advantage of chemically modifying the material is to facilitate continuous sterilization during use, which would decrease the potential for aerosolized fomites when using or removing PPE, thereby decreasing a potential mode of infection 10 .
To differentiate the impact that immobilized 3 and visible light contribute to the viral inactivation efficacy, we completed an analogous virus exposure test of SBPP-3 in the absence of light (Fig. 3b). Without exposure to light, SBPP-3 minimally inactivated the inactivated the virus with a 0.76 log reduction ( Fig. 3b; SBPP-3 Dark), which was substantially less than SBPP exposed to light. These data indicated that immobilized 3 and visible light are required to achieve efficient virus inactivation, and that switchable on/off performance and lithography/ patterning of virus inactivation may be possible with this system.
To confirm the presence and quantity of the sensitized molecular species-1 O 2 and ROS-responsible for inactivating the viruses upon exposure to white light, a selective scavenging experiment utilizing p-nitrosoaniline (pNDA) was employed (see Method section for details) 38 . pNDA bleaching by ROS can be quantified spectrophotometrically by the reduction of absorbance of pNDA at 440 nm ; comparatively, 1 O 2 is not capable of bleaching pNDA directly. Utilizing a combination of pNDA and imidazole-with the imidazole capable of reacting efficiently with 1 O 2 to produce an intermediate species capable of bleaching pNDA-the quantification of 1 O 2 can then be determined through the reduction of the absorbance of pNDA at 440 nm in comparison to the ROS specific experiment above. White light exposure of SBPP-3 in combination with pNDA (scavenging ROS) or pNDA + imidazole (scavenging ROS and 1 O 2 ) for a duration of 10, 100, and 1000 min was completed and analyzed by UV-Vis spectroscopy at 440 nm and plotted as a change in concentration of pNDA vs. exposure time (Fig. 3c). The results indicated that in the presence of light SBPP-3 primarily generates 1 O 2 and not other ROS. Additionally, to probe the stability of the photosensitizer over longer periods of white light exposure, a sample of SBPP-3 was exposed to high intensity white light for 4 days, and then underwent an analogous 1000-min www.nature.com/scientificreports/ 1 O 2 quantification experiment (white light + pNDA + imidazole); the results indicated the material had a similar level of 1 O 2 production, albeit with a larger standard deviation (Fig. 3c, labelled as pre-exposure at 1000 min). Lastly, the effect of functionalization on filtration efficiency was tested using MBPP-3; SBPP materials are typically the outer and inner coverings on masks and do not possess a high degree of filtration (below 10% filtration efficiencies below 2 µm particles) whereas MBPP materials have a higher density of thinner diameter fibers that enable higher filtration efficiencies with multiple layers. Filtration efficiency of pristine MBPP was compared to MBPP-3 and MBPP that underwent an analogous procedure, exclusive of additive 3-denoted MBPP MeOH . The MBPP-3 and MBPP MeOH had equivalent filtration efficiencies, indicating that the photosensitizer 3 had no negative effect on filtration performance (Fig. 3d). The decrease in filtration performance of MBPP MeOH and MBPP-3 in comparison to MBPP was caused by the elimination of the electrostatic charge; methods to regenerate the electrostatic charge on the filters have been explored by others with success and provides a possible method if post-production functionalization is utilized 37 .
The ability to functionalize aliphatic polymers with diazirines is a relatively new methodology and has the potential to impact a large portion of the commodity polymer market. Low-functionality aliphatic polymerssuch as the SBPP/MBPP used in this research-account for the largest three (polypropylene, low-density and high-density polyethylene) volumes of thermoplastics in the world equating to ~ 36% or 23 million tons of polymers used worldwide each year 34 . With over 39% in packaging and 22% in other areas that include health and safety, the potential for improvement in product performance and safety across different markets that utilize aliphatic polymers is high. Furthermore, this method of functionalization can be applied to different commodity polymers including polystyrene, polyurethane, polyethylene terephthalate, nylon, and acrylic and as such may allow recycled materials an avenue for use in high-performance and advanced material applications from renewable resources 39 . The diazirine functionality is not limited to C-H bond activation and can also be used to functionalize more reactive O-H and N-H bonds in polyalcohols and polyamides which could be used for post-processing functionalization of different materials that would benefit from self-sterilization in healthcare settings 30 .
Future testing will focus on the development of this technology to understand the performance limitations of the material with respect to photosensitizer loading and surface coverage, repeated sequential virus inactivation, potential photobleaching, light intensity-dependent performance, response to washing and detergents, and performance against different types of pathogens. The optimization of inactivation materials should be focused www.nature.com/scientificreports/ on developing technology that is broadly applicable, robust, and possesses broad spectrum activity without the potential for developing resistance.

Conclusions
We have described the production of a polypropylene-based non-woven filter that was covalently functionalized with a zinc-porphyrin photosensitizer using diazirine C-H activation chemistry. The MBPP-3 material was tested against a model virus, Influenza A, to explore the virus inactivation abilities of the material when exposed to visible light. Over a 4-h incubation period with exposure to visible light there was 4-log reduction of active virus resulting in a logarithmic trend in the inactivation of virus over time, and a 5.95 log reduction in comparison to the starting virus titer. This research presents a new approach to achieving functionalized aliphatic polymers, such as those used in PPE, which provides a potential solution for reducing pathogen transfer; a route for designing re-useable and re-sterilizable PPE that can reduce the need for single-use products; and the development of post-functionalization processes that could see widespread use across many different forms of PPE.

Methods
All chemicals were used as received.  Production of zinc porphyrin functionalized spunbond and meltblown polypropylene (SBPP-3 and MBPP-3, respectively). SBPP or MBPP was cut into 4 cm diameter circles (with an initial white colour) and placed in 4 cm diameter aluminum weigh boats. Each filter piece was submerged in a methanol solution of 3 (equating to a concentration of 3 that was 10 wt% of the SBPP or MBPP textile) and was subsequently covered with aluminum foil and allowed to incubate at room temperature for 1 h. The aluminum pans containing the SBPP or MBPP and 3 were then uncovered and the methanol solvent was allowed to evaporate in the dark for 4 h which resulted in a green coloured SBPP or MBPP textile. The pans containing SBPP or MBPP and 3 were then incubated for 4 h at 120 °C in an oven. The resulting SBPP-3 and MBPP-3 textile was then washed with ethanol to remove any residual non-bound 3 by incubating the textile in 10 mL (first 10 washings) then 500 mL (last two washings) of ethanol until no remaining 3 was observed by UV-Vis spectroscopy. The SBPP-3 and MBPP-3 textiles were then air dried and used for virus inactivation testing, 1  www.nature.com/scientificreports/ were split into aliquots and stored at − 80 ℃ until use. Virus titers were determined by plaque assay. In brief, virus samples were serially diluted tenfold in DMEM. Madin-Darby Canine Kidney cell monolayers (ATCC) in 6-well plates were inoculated with 200 µL of virus at each dilution in triplicate. After 1 h adsorption at 37 ℃, the inoculum was removed and the monolayers were overlaid with DMEM containing 1% Noble Agar and 0.0075% trypsin. After incubation at 37 ℃ for 48 h, plaques were stained with neutral red and counted. Antiviral efficacy was calculated by comparing the number of resultant plaques.